Research Article  Open Access
B. Merckx, P. Dudoignon, J. P. Garnier, D. Marchand, "Simplified Transient HotWire Method for Effective Thermal Conductivity Measurement in Geo Materials: Microstructure and Saturation Effect", Advances in Civil Engineering, vol. 2012, Article ID 625395, 10 pages, 2012. https://doi.org/10.1155/2012/625395
Simplified Transient HotWire Method for Effective Thermal Conductivity Measurement in Geo Materials: Microstructure and Saturation Effect
Abstract
The thermal conductivity measurement by a simplified transient hotwire technique is applied to geomaterials in order to show the relationships which can exist between effective thermal conductivity, texture, and moisture of the materials. After a validation of the used “one hotwire” technique in water, toluene, and glassbead assemblages, the investigations were performed (1) in glassbead assemblages of different diameters in dried, water, and acetonesaturated states in order to observe the role of grain sizes and saturation on the effective thermal conductivity, (2) in a compacted earth brick at different moisture states, and (3) in a limehemp concrete during 110 days following its manufacture. The limehemp concrete allows the measurements during the setting, desiccation and carbonation steps. The recorded diagrams allow the calculation of one effective thermal conductivity in the continuous and homogeneous fluids and two effective thermal conductivities in the heterogeneous solids. The first one measured in the short time acquisitions (<1 s) mainly depends on the contact between the wire and grains and thus microtexture and hydrated state of the material. The second one, measured for longer time acquisitions, characterizes the mean effective thermal conductivity of the material.
1. Introduction
The thermal and hydric transfers in geomaterials are fundamental phenomena which can govern firstly the comfort in buildings and residences and secondly the durability of the materials. The microclimatic simulations of the hygrometric and thermal conditions prevailing in the building interiors need the estimation of the wall material characteristics: moisture and effective thermal conductivity face to the outer climatic changes. In fact, the thermal and hydric conductivities are intrinsic properties of the materials. The heat transfers mainly depend on the frequency of grain contacts, size of pores, and airwater ratio infilling the porosity. The moisture transfers mainly depend on the connectivity associated to the mesotomicro porosity distribution. The development and implementation of “ecomaterials” for building have to demonstrate their ecologic qualities both by their productions and building techniques and also by their thermal and hydric insulation properties. In this “ecomaterial” domain, the earth material and concretes using plant fibers as aggregates are more and more used. Their uses are governed by their mechanical and thermal properties, that is, minimum of mechanical resistance face to the construction necessities and insulation or heat storage abilities. The building techniques of earth material have been largely discussed and normalized. The material cohesion is assumed by the clay mineral matrix often added of some percents of lime or cement. The mechanical resistances are due (1) to the clay matrix cohesion which acts as cement between the sand grains and (2) to the compactness of the claysand assemblage which decreases the volume of microporosity. This compactness of the material influences the mesotomicro porosity distribution. The concretes using plant fibers as aggregates are more and more used with increasing cementtolime replacement. These new cement or limeplant fiber concretes are mainly appreciated for their small effective thermal conductivities. Nevertheless, the thermal conductivities evolve with time according to the structure and saturation index evolutions of the material during the setting, desiccation, and carbonation steps.
The THW method has been progressively developed from 1931 until now [1, 2]. The method has been particularly advanced these last forty years thanks to very accurate measurements, firstly due to two wires, electric bridges, and smallsize devices and secondly due to finiteelement simulations [2–5]. The THW method has been used for pure phases as gas, liquids [3, 6–11], solids, and melts [4, 5]. The method was also developed for measurements in electroconducting and in highly corrosive liquids [12–15]. Actually, although the guarded hot plate technique is largely used, the transient hotwire method is extended to the measurement and calculation of the effective thermal conductivity of granular materials [16–19], rocks [20–22], building materials, [23–25], and soils [26–28] via multicaptor or multineedle probes.
The objective of the work is to show that a transient hotwire (THW) technique, simplified to only one hotwire embedded in geomaterials, allows rapid characterization on the thermalhydric properties of the building materials which remain realistic face to their heterogeneity. The texturemoisture and thermal effective conductivity relationships are studied firstly on glassbead assemblages of different diameters in order to demonstrate the role of grain size and saturation index. Secondly, the measurements have been performed in materials used for “ecoconstruction,” that is, sand + clay matrix compacted material (compacted earth brick) and limehemp concrete in order to follow the evolution of the effective thermal conductivity during their maturation. The technique is tested in such very thin divided and microporous materials taking into account the moisture evolution due to the desiccation and structure evolutions.
2. Method and Materials
2.1. Principle of the THW Method
The THW method is a transient dynamic technique based on the measurement of the temperature rise of a linear heat source (hot wire) embedded in the tested material [2, 7–15]. For an infinitely long metallic wire (length/radius ratio ≫200) heated at time with a constant heat flux per length unit and immersed in an infinite homogeneous medium (thermal conductivity and diffusivity: and , resp.) with uniform initial temperature, the temperature rise of the wire is given by (1) [29]: with where is Euler’s constant and Fo the Fourier number defined by
Equation (1) is the analytical solution of an ideal thermal conductive model valid for and without convective transfers [2, 3, 16].
From this ideal model and with known values, the thermal conductivity can be calculated by where is a numerical constant deduced from experimental data for values which satisfy the condition .
For practical applications of the THW method, wire and material sample dimensions, among other ideal model hypothesis, are finite and the deviations from the ideal model have then to be evaluated. In fact, the answer to the wire heating resultant of the Joule effect due to an electrical current is with the instantaneous electrical resistance of the wire, the resistance of the wire at the reference temperature, and the temperature coefficient of the wire at 22°C.
Taking into account (3) and (4), the thermal conductivity may be calculated as follows: where is a numerical constant deduced from the experimental data and from the linear part of the curve.
2.2. Materials
The heat transfers were measured in assemblages of glass beads and in two geomaterials, that is, a compacted earth brick and a limehemp concrete brick. The data (temperature versus time) were recorded using a very pure Ni (>99.98%) wire of 0.125 mm diameter insert in the glassbead assemblages or in the earth brick and limehemp brick during the manufacture (Figure 1). The choice of.125 mm diameter of the Ni wire was motivated by the length/diameter ratio in order to minimize the end effect, and by the necessary wire resistance face to the manufacturing processes. The heat transfers were induced by constant heating using 100 mA or 300 mA current. The current generator has to be very precise. It is a Keithley 2400 (precision of 10^{−6} A). The nanovoltmeter used is a Keithley 2182 (precision of 10^{−8} V). The experiments are driven by a microcomputer equipped with GPIB connections and Labview software. All the measurements are made using the four wire technique.
(a)
(b)
(c)
Successive glassbead media have been tested. Three types of glass beads Sili S, SL, and M are used. They differ by weak differences in chemical compositions and associated densities (Table 1). Each bead assemblage is characterized by a grain size range d–D evolving from 1.50–1.70 mm in diameter to 3.80–4.10 mm for the type M, from 0.40–0.60 mm to 3.75–4.50 mm for the type S, and from 0.50–0.80 mm to 2.50–3.20 mm for the type SL. In spite of the differences in the d–D ranges, the porosity of the successive dead assemblages shows small differences that is, 0.37, 0.39, and 0.39 mean porosities for the M, S, and SL bead assemblages, respectively. To make evident the effect of saturation, the 2.8–3.4 mm glassbead medium has also been tested saturated with water and acetone. All the glassbead media have been tested in dried state. The dimensions of the cylindrical cell filled by the glass beads are 19.8 cm height and 7 cm diameter (Figures 1(a) and 1(b)).

The compacted earth brick is made by mechanical compression of earth plus sand mixture added of 5% lime. In weight percentage, the composition of the compacted brick is 62% earth, 28% sand, 5% lime, and 5% water. The dimensions of the bricks are 29.5 cm length, 14 cm width, and 9.5 cm height (Figure 1(c)). The mineralogy of sand is quartz dominant, feldspars, and accessory Fe oxides. The mineralogy of the clayey fraction in earth is Illite, Kaolinite, and Smectite. The effective thermal conductivity is measured in the compacted brick from its initial 17% of gravimetric water content to 3% of residual water content after 110 days of air drying. The 17% of water content correspond to a saturation index () of 90%. The 3% of water content correspond to a saturation index of 15%. The measurements were made daily during the first sixty days and with larger steps (23 days) after (Figures 7 and 9).
The limehemp concrete is composed of mixture of 25 kg water, 5.08 kg (60 L) hemp (chenevotte), and 35 kg lime. The weight formulae of the limehemp concrete evolve from 38.5% of water, 7.8% of chenevotte, and 53.8% of lime for the fresh concrete. The percentage in weight of lime increases to 76% for mature concrete. The lime is a Batichanvre Saint Astier (NHL5). The dimensions of the earth and limehemp bricks are 29.5 cm length, 14 cm width, and 9.5 cm height (Figure 1(c)).
The heat transfer measurements are represented in versus diagrams (Figures 2 and 3). Two types of versus curves are obtained: the “oneslope” curve characteristic of a continuous wiremedium contact observed for liquids (Figure 2), and the “twoslopes” curves observed for the granular media (Figure 3). For the glass beads and the earth brick, the “twoslopes” curves accord to two successive steps of temperature increasing characterized by and slopes, respectively. The and slopes are used to calculate two associated thermal conductivities and as follows ((6); Figure 2): with the curve slope , the electrical resistance of the wire, the current intensity, the wire length.
(a)
(b)
(a)
(b)
(c)
This one hotwire probe was firstly validated by measurements in water and toluene (22°C). Ten successive measurements give water and toluene thermal conductivities of 0.602 W/mK and 0.1313 W/mK, respectively, in good agreement with bibliographic data [6]. The ten successive measurements give a standard deviation of 0.008 W/mK for the water and 0.002 W/mK for the toluene. These ones are equivalent to 1.33% and 1.5% and argue for a good repeatability of the measurements (Figure 2). Repeatability tests have also been made on a glassbead assemblage (M 2 mm diameter). The results give 0.048 W/mK with a 0.001 W/mK standard deviation (2%) for , and 0.277 W/mK with 0.004 W/mK standard deviation (1.44%) for (Figure 3).
The short time slope is characteristic of the noncontinuous wiremedium contact [30, 31]. For the measurement of thermal conductivity of solids, this contact artifact is often reduced by the addition of a continuous thin layer of transition material as gel, for example [4, 5]. In fact, in this work, we try to use this slope to get characteristics on the texture and saturation index of our granular materials.
The precision of the measurements is influenced by many sets. The precisions of the generator (10^{−6} A) and of the nanovoltmeter (10^{−8} V) minimize a cumulate error on the measurement which is inferior to 0.01%. Estimating an error of wire length measurement of 0.5 mm, the induced error of measurement is 0.5%. The end effect error can be calculated following Knibbe’s equation [32] taking into account the wire radius/length ratio, the material/wire thermal conductivities, and material diffusivity. Using 125 μm diameter Ni wire of 19.8 cm in the glassbead assemblages and 29.5 cm length in the earth and lime brick, the errors are 1.5%, 0.6%, and 1.2% respectively. Taking into account all these sources of error, the cumulated one is inferior to 3%.
3. Results
3.1. Glass Beads
For the glassbead materials, all the curves show the same features: a first rapid increase in short time (<1 s) and slow increase for time >1 s (Figure 4). These two domains are characterized by two and slopes, respectively. In the shorttime domain, increases when the bead diameter increases. In fact, the slope depends on the density of bead contacts with the wire. The associated evolves from 0.11 W/mK to 0.038 W/mK. It can be expressed as a function of the bead diameter (mm) as follows ((7); Figure 5(a)):
(a)
(b)
For the successive tests performed on the different materials, the diameter relationship follows a weak and linear evolution ((8); Figure 4(b)):
The two obtained and characterize the “microstructural” and the effective thermal conductivities of the bead assemblages, respectively. The “microstructural” effect is reached thanks to the 0.125 mm wire diameter. In order to quantify the influence of the porosity saturation the measurements were performed on the dried “air saturated,” acetonesaturated and watersaturated material (Tables 2 and 3).


The measurements for the different saturation states were made on the 2.8–3.4 mm diameter glassbead assemblages. Three types of curves were obtained (Figure 6; Table 3):(i)the curve characteristic of the dried bead assemblage with the two successive and characteristics of the microstructure and of the whole material,(ii)a very flat curve two slope curve for the acetone saturation,(iii) a straight line for the water saturation.
The measured in our glassbead assemblages accord with the data of Kohout et al. [33] obtained on glass beads of 200 μm diameters with glass thermal conductivity of 0.80 W/mK and an assemblage porosity of 0.39. He obtained an effective thermal conductivity increasing from 0.15 W/mK in dried state to 0.73 W/mK in watersaturated state. For similar conditions, the effective thermal conductivities calculated with the Maxwell model give 0.175 W/mK and 0.815 W/mK, respectively [16]. This increase according to the saturation index holds also with the Jougnot and Revil results [20] and with the Maxwell and Ktupiczka simulations [16, Table 3].
3.2. Compacted Earth Brick
The thermal conductivities were measured during the 110 days of the brick desiccation. The manufacturing of the earth brick by mechanical compression induced a quite saturated material initially characterized by a saturation index () of 90%. The progressive desiccation causes the simultaneous decrease of the water content and saturation index, from 17 to 3% and 90 to 15%, respectively (Figure 7).
For this material, only one brick and, consequently, only one texture was tested. The sand grains are coated by the earth clay material. In fact, the claytosand skeleton and the small initial porosity of the compacted material have limited the shrinkage phenomenon. Thus, the porosity may be counted as constant during the desiccation and mainly assumed by the clay matrix microporosity. The scanning electronic microscope confirms this microstructure of the compacted brick. The clay matrix is very compact. All the porosity is constituted of microporosity disseminated between the clay particles and almost micropores have sizes lower than 20 μm (Figure 8).
Nevertheless, the curves show evolutions from saturated to unsaturated states which are similar to the glassbead assemblage ones, that is, a first step of rapid increase in short time (<1 s) and a second one of slow increase for time >1 s. The successive curves are only dependent of the water content and the saturation index. In these conditions, for invariant texture of the material, the evolutions of and during the drying period characterize the decrease of moisture. The first curves recorded during the first week show quite flat patterns. On the contrary, the curves recorded at the end of the drying period (110 days) show clearly the two different and slopes (Figure 9). The first curves were recorded for saturation index near 90% and the last measurement series were performed for saturation index of 15%. This evolution of the curve patterns has consequences on the calculated thermal conductivity (Figures 10 and 11): drastic decrease of for high water content and associated high (50 to 90%), and weak decrease for <50%. The is quite constant whatever the water content is.
The evolutions of and measured on the earth brick show parallel decrease from the saturated initial state to the 0.65 saturation index (10 days): that is, from 0.94 to 0.50 W/mK and 1.17 to 0.97 W/mK, respectively. For lower saturation index, the values present dispersion around a 0.97 W/mK mean value with a standard deviation of 0.05 W/mK (5%). On the contrary, from the saturated state to low saturation index, the values show a continuous decrease from 0.94 to 0.09 W/mK following a fitted polynomial curve: , with . This versus curve may be used as a good indicator of the material moisture. The comparison with the Cox clay rock of Jougnot and Revil [20] shows similar decrease of the values from the dried state to saturated one. Nevertheless, its data characterized the effective thermal conductivity of the rock in a low porosity domain (0.14to0.16). The 2.0 to 1.41 W/mK decrease of measured in the Cox clay rock is comparable with the 1.17 to 0.95 W/mK decrease of measured in the 100 to 0.65 domain for our earth brick with a porosity of 0.30.
3.3. LimeHemp Concrete
Two days were necessary to allow the removal of the test piece from the mould. The measurements by the THW method began 2 days after the manufacturing of the limehemp concrete. The weight of the test piece was measured from 2 to 110 days. The relative lost of weight was 42.10%. It includes the lost of water by desiccation, the hydration, and the carbonation of the lime. The curve of weight versus time shows a “hyperbolic” shape characterized by (Figure 12)(i) a very high weight lost (170 g/day equivalent to 4.47%/day) during the 8 first days,(ii) a weight decrease following a exponential law from 8 to 55 days; that is,(iii) a low decrease from 55 to 110 days (2 g/day equivalent to 0.05%/day).
The successive recorded curves differ from the glass beads and earth brick ones by their staight line shapes. Only the first 0 to 0.3 second measurements do not bring into alignement with the whole data. Nevertheless, the slopes of straight lines increase with the lost of water, following the same trends as the clayrich compacted brick (Figure 13).
The obtained oneslope curve suggests the subcontinuous lime past—wire contact. According to the straightline shape of the curves, only one can be calculated.
The evolution with time accords to the lost of weigth which may be simplified as a lost of water content. Two steps are evident in the diagram. They are characterized by two linear relationships (Figure 14):(i)0 to 20 days; ,(ii)20 to 110 days; .
The final tends to 0.29 W/mK.
4. Discussions and Conclusion
The investigations, using only one hot wire, in spite of its simplicity and basic aspect face to the recent developments, were tested on granular and geomaterials. Despite the measurement precisions lower than those obtained on pure phases by recent investigations (3% against 1% for Assael et al. results; [4, 5]), this one seems to be overestimated face to the 1.5% experimental error obtained on the water and toluene. Nevertheless, the following conditions are necessary to minimize the measurement errors:(i)the diameter/length ratio of wire has to be very small to allow the simplification as infinite linear wire, according to the theory. Nevertheless, it has to be appropriated to the manufacture of the test pieces that is; very low end effect error and sufficient resistance of the embedded wire face to the eventual compression of the material in moulds,(ii)a very accurate measurement of the wire length and of the associated currents and voltages.
In order to avoid all the artifacts of material surface/wire contact, the hot wires were embedded into the materials during their manufactures. The wire insertion is particularly easy for the glassbead assemblages and during the earth brick or limehemp concrete compaction, and, therefore, for different other types of manufactured geomaterials. The experiments on glass beads show the interest in recording the patterns in short (<1 s) and long acquisition times. In short times, the patterns allow characterisations on the microstructure and the saturation state of the material. The measurements on the clay dominant material show similar results in spite of the very thin size of particles and associated microporosity. The evolution of the coefficient obtained in short times is sufficient to characterize the moisture and saturation index of the material for one knew grain size distribution (Figures 4 and 5). The coefficient obtained during the second step of acquisition ( s) is characteristic of the whole material effective thermal conductivity. In addition, the and are commensurate with the grain size of the material (Figure 5).
Tested on the limehemp concrete from its manufacture to advance desiccation + setting steps (110 days), the method confirms its validity for geomaterials. The curves evolve according to the desiccation + setting advancement. Nevertheless, the curves present straightline patterns which allow the calculation of only one thermal conductivity characteristic of the whole material. The lack of the first slope, of the curve, equivalent to the “short time” results of the continuous coating of the wire by the lime cement.
These preliminary results suggest the possibility of investigation on the relationship which prevails between the microstructure and saturation state of geomaterials and their effective thermal conductivity. The technique may be extended to in situ measurements in walls, soils, and other materials in order to record data on the thermohydric transfers and to be used for the mathematical simulations of the mechanisms.
References
 M. J. Assael, K. D. Antoniadis, and W. A. Wakeham, “Historical evolution of the transient hotwire technique,” International Journal of Thermophysics, vol. 31, no. 6, pp. 1051–1072, 2010. View at: Publisher Site  Google Scholar
 J. J. Healy, J. J. de Groot, and J. Kestin, “The theory of the transient hotwire method for measuring thermal conductivity,” Physica B+C, vol. 82, no. 2, pp. 392–408, 1976. View at: Google Scholar
 “Measurement of the transport properties of fluids,” in Experimental Thermodynamics, W. A. Wakeham, A. Nagashima, and J. V. Sengers, Eds., vol. 3, Blackwell Scientific Publications, London, UK, 1991. View at: Google Scholar
 M. J. Assael, K. D. Antoniadis, and J. Wu, “New measurements of the thermal conductivity of PMMA, BK7, and Pyrex 7740 up to 450K,” International Journal of Thermophysics, vol. 29, no. 4, pp. 1257–1266, 2008. View at: Publisher Site  Google Scholar
 M. J. Assael, K. D. Antoniadis, K. E. Kakosimos, and I. N. Metaxa, “An improved application of the transient hotwire technique for the absolute accurate measurement of the thermal conductivity of pyroceram 9606 up to 420 K,” International Journal of Thermophysics, vol. 29, no. 2, pp. 445–456, 2008. View at: Publisher Site  Google Scholar
 M. L. V. Ramires, J. M. N. A. Fareleira, C. A. Nieto de Castro, M. Dix, and W. A. Wakeham, “The thermal conductivity of toluene and water,” International Journal of Thermophysics, vol. 14, no. 6, pp. 1119–1130, 1993. View at: Publisher Site  Google Scholar
 J. R. Parsons Jr. and J. C. Mulligan, “Measurement of the properties of liquids and gases using a transient hotwire technique,” Review of Scientific Instruments, vol. 49, no. 10, pp. 1460–1463, 1978. View at: Publisher Site  Google Scholar
 C. A. Nieto De Castro, J. C. G. Calado, W. A. Wakeham, and M. Dix, “An apparatus to measure the thermal conductivity of liquids,” Journal of Physics E, vol. 9, no. 12, article 020, pp. 1073–1080, 1976. View at: Publisher Site  Google Scholar
 R. A. Perkins, M. L. V. Ramires, and C. A. Nieto De Castro, “Thermal conductivity of saturated liquid toluene by use of anodized tantalum hot wires at high temperatures,” Journal of Research of the National Institute of Standards and Technology, vol. 105, no. 2, pp. 255–265, 2000. View at: Google Scholar
 R. A. Perkins, M. L. V. Ramires, C. A. Nieto de Castro, and L. Cusco, “Measurement and correlation of the thermal conductivity of butane from 135 K to 600 K at pressures to 70 MPa,” Journal of Chemical and Engineering Data, vol. 47, no. 5, pp. 1263–1271, 2002. View at: Publisher Site  Google Scholar
 G. Thevenot, J. Saillard, J. P. Maye, and J. P. Garnier, “Cellule de mesure de la conductivité et de la diffusivité thermiques d’un fluide et sonde pour cette cellule,” European Patent Office. EP 1724572 A1, 2006. View at: Google Scholar
 A. Alloush, W. B. Gosney, and W. A. Wakeham, “A transient hotwire instrument for thermal conductivity measurements in electrically conducting liquids at elevated temperatures,” International Journal of Thermophysics, vol. 3, no. 3, pp. 225–235, 1982. View at: Publisher Site  Google Scholar
 Y. Nagasaka and A. Nagashima, “Absolute measurement of the thermal conductivity of electrically conducting liquids by the transient hotwire method,” Journal of Physics E, vol. 14, no. 12, pp. 1435–1440, 1981. View at: Publisher Site  Google Scholar
 J. P. Garnier, J. P. Maye, J. Saillard, G. Thévenot, A. Kadjo, and S. Martemianov, “A new transient hotwire instrument for measuring the thermal conductivity of electrically conducting and highly corrosive liquids using small samples,” International Journal of Thermophysics, vol. 29, no. 2, pp. 468–482, 2008. View at: Publisher Site  Google Scholar
 A. Kadjo, J. P. Garnier, J. P. Maye, and S. Martemianov, “A new transient twowire method for measuring the thermal diffusivity of electrically conducting and highly corrosive liquids using small samples,” International Journal of Thermophysics, vol. 29, no. 4, pp. 1267–1277, 2008. View at: Publisher Site  Google Scholar
 I. H. Tavman, “Effective thermal conductivity of granular porous materials,” International Communications in Heat and Mass Transfer, vol. 23, no. 2, pp. 169–176, 1996. View at: Publisher Site  Google Scholar
 J. Z. Liang and F. H. Li, “Measurement of thermal conductivity of hollow glassbeadfilled polypropylene composites,” Polymer Testing, vol. 25, no. 4, pp. 527–531, 2006. View at: Publisher Site  Google Scholar
 E. E. Gonzo, “Estimating correlations for the effective thermal conductivity of granular materials,” Chemical Engineering Journal, vol. 90, no. 3, pp. 299–302, 2002. View at: Publisher Site  Google Scholar
 G. K. Batchelor and R. W. O'Brien, “Thermal or electrical conduction through a granular material,” Proceedings of the Royal Society of London Series A, vol. 355, no. 1682, pp. 313–333, 1977. View at: Google Scholar
 D. Jougnot and A. Revil, “Thermal conductivity of unsaturated clayrocks,” Hydrology and Earth System Sciences, vol. 14, no. 1, pp. 91–98, 2010. View at: Google Scholar
 C. Gruescu, A. Giraud, F. Homand, D. Kondo, and D. P. Do, “Effective thermal conductivity of partially saturated porous rocks,” International Journal of Solids and Structures, vol. 44, no. 34, pp. 811–833, 2007. View at: Publisher Site  Google Scholar
 J. P. Cull, “Thermal conductivity probes for rapid measurements in rock,” Journal of Physics E, vol. 7, no. 9, article 026, pp. 771–774, 1974. View at: Publisher Site  Google Scholar
 M. Stefanidou, M. Assael, K. Antoniadis, and G. Matziaroglou, “Thermal conductivity of building materials employed in the preservation of traditional structures,” International Journal of Thermophysics, vol. 31, no. 45, pp. 844–851, 2010. View at: Publisher Site  Google Scholar
 A. Bouguerra, “Temperature and moisture dependence on the thermal conductivity of woodcementbased composite: experimental and theoretical analysis,” Journal Physics D.: Applied Physics, vol. 32, no. 21, pp. 2797–2803, 1999. View at: Publisher Site  Google Scholar
 A. Bouguerra, A. Ledhem, F. De Barquin, R. M. Dheilly, and M. Quéneudec, “Effect of microstructure on the mechanical and thermal properties of lightweight concrete prepared from clay, cement, and wood aggregates,” Cement and Concrete Research, vol. 28, no. 8, pp. 1179–1190, 1998. View at: Google Scholar
 K. L. Bristow, “Measurement of thermal properties and water content of unsaturated sandy soil using dualprobe heatpulse probes,” Agricultural and Forest Meteorology, vol. 89, no. 2, pp. 75–84, 1998. View at: Publisher Site  Google Scholar
 K. L. Bristow, G. J. Kluitenberg, C. J. Goding, and T. S. Fitzgerald, “A small multineedle probe for measuring soil thermal properties, water content and electrical conductivity,” Computers and Electronics in Agriculture, vol. 31, no. 3, pp. 265–280, 2001. View at: Publisher Site  Google Scholar
 D. A. De Vries and A. J. Peck, “On cylindrical probe method of measuring thermal conductivity with special reference to soils,” Australian Journal of Physics, no. 11, pp. 225–271, 1958. View at: Google Scholar
 H. S. Carslaw and J. C. Jaeger, Conduction of Heat in Solids, Oxford University Press, London, UK, 1959.
 A. Testu, Dispersion thermique dans des milieux granulaires: caractérisation à cœur et en proche paroi, thèse, Institut National Polytechnique de Lorraine, Nancy, 2005.
 H. Martin, “Low peclet number particletofluid heat and mass transfer in packed beds,” Chemical Engineering Science, vol. 33, no. 7, pp. 913–919, 1978. View at: Google Scholar
 P. G. Knibbe, “The endeffect error in the determination of thermal conductivity using a hotwire apparatus,” International Journal of Heat and Mass Transfer, vol. 29, no. 3, pp. 463–473, 1986. View at: Google Scholar
 M. Kohout, A. P. Collier, and F. Stepanek, “Effective thermal conductivity of wet particle assemblies,” International Journal of Heat and Mass Transfer, vol. 47, no. 25, pp. 5565–5574, 2004. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2012 B. Merckx et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.